#------------------------------------------------------------------------------
#$Date: 2017-02-07 17:13:06 +0200 (Tue, 07 Feb 2017) $
#$Revision: 191892 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103531.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103531
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.54 La3 O14 Ta0.46'
_chemical_formula_weight         1110.22
_chemical_name_systematic        ?
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   8.158
_cell_length_b                   8.158
_cell_length_c                   5.099
_cell_measurement_temperature    293(2)
_cell_volume                     293.9
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         3.0E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.338
_diffrn_measured_fraction_theta_max 0.338
_diffrn_radiation_source         synchrotron
_diffrn_radiation_wavelength     0.56000
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0504
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            759
_diffrn_reflns_theta_full        38.48
_diffrn_reflns_theta_max         38.48
_diffrn_reflns_theta_min         2.27
_exptl_absorpt_coefficient_mu    14.499
_exptl_crystal_density_diffrn    6.273
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             488
_refine_diff_density_max         2.579
_refine_diff_density_min         -2.144
_refine_diff_density_rms         0.443
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.16(7)
_refine_ls_extinction_coef       0.023(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.138
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         759
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.138
_refine_ls_R_factor_all          0.0400
_refine_ls_R_factor_gt           0.0389
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1249
_refine_ls_wR_factor_ref         0.1364
_reflns_number_gt                756
_reflns_number_total             759
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-3d3.cif
_cod_data_source_block           3d3
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

Changing (with the help of Perl) all _diffrn_radiation_source values in
the files that were reportedly colected on the HASYLAB D3 beamline
(Hamburg) from 'fine-focus sealed tube' to synchrotron.

The command was:

perl -i -ne \
    "s/'fine-focus sealed tube'/synchrotron/; \
    print unless /_diffrn_radiation_type|_diffrn_radiation_monochromator/" \
    *d3*.cif \
    11.57split.cif \
    21.85split.cif \
    22.85split.cif

Saulius Gra\<zulis
;
_cod_database_code               2103531
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La -0.42713(10) 0.0000 0.0000 0.00852(17) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0078(3) Uani 0.50 6 d SP
Ta Ta 0.0000 0.0000 0.0000 0.0078(3) Uani 0.50 6 d SP
Ga2 Ga -0.6667 -0.3333 0.4694(4) 0.0077(3) Uani 1 3 d S
Ga3 Ga -0.7634(2) 0.0000 -0.5000 0.0101(3) Uani 1 2 d S
O1 O -0.3333 0.3333 0.178(2) 0.0042(16) Uani 1 3 d S
O2 O -0.1491(12) 0.3077(15) -0.3031(17) 0.0157(17) Uani 1 1 d .
O3 O -0.1439(13) 0.0749(14) 0.2404(14) 0.0153(16) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.9400 1.6200 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.9400 4.4000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2490 1.0600 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0028 0.0036 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 67.3(4) 6 .
O3 La O2 139.5(3) 6 2_455
O3 La O2 107.7(3) . 2_455
O3 La O2 107.7(3) 6 4_455
O3 La O2 139.5(3) . 4_455
O2 La O2 100.5(4) 2_455 4_455
O3 La O1 79.2(2) 6 2_455
O3 La O1 124.7(2) . 2_455
O2 La O1 71.5(3) 2_455 2_455
O2 La O1 91.4(2) 4_455 2_455
O3 La O1 124.7(2) 6 .
O3 La O1 79.2(2) . .
O2 La O1 91.4(2) 2_455 .
O2 La O1 71.5(3) 4_455 .
O1 La O1 153.50(6) 2_455 .
O3 La O2 66.2(3) 6 .
O3 La O2 79.2(3) . .
O2 La O2 154.31(14) 2_455 .
O2 La O2 63.4(4) 4_455 .
O1 La O2 125.7(3) 2_455 .
O1 La O2 65.1(2) . .
O3 La O2 79.2(3) 6 6
O3 La O2 66.2(3) . 6
O2 La O2 63.4(4) 2_455 6
O2 La O2 154.31(14) 4_455 6
O1 La O2 65.1(2) 2_455 6
O1 La O2 125.7(3) . 6
O2 La O2 138.4(3) . 6
O3 La Ga2 110.5(2) 6 .
O3 La Ga2 86.5(2) . .
O2 La Ga2 31.1(2) 2_455 .
O2 La Ga2 129.3(2) 4_455 .
O1 La Ga2 65.1(2) 2_455 .
O1 La Ga2 109.9(2) . .
O2 La Ga2 165.54(17) . .
O2 La Ga2 32.38(17) 6 .
O3 La Ga2 86.5(2) 6 2_565
O3 La Ga2 110.5(2) . 2_565
O2 La Ga2 129.3(2) 2_455 2_565
O2 La Ga2 31.1(2) 4_455 2_565
O1 La Ga2 109.9(2) 2_455 2_565
O1 La Ga2 65.1(2) . 2_565
O2 La Ga2 32.38(17) . 2_565
O2 La Ga2 165.54(17) 6 2_565
Ga2 La Ga2 159.92(3) . 2_565
O3 La Ga1 33.66(18) 6 .
O3 La Ga1 33.66(18) . .
O2 La Ga1 129.7(2) 2_455 .
O2 La Ga1 129.7(2) 4_455 .
O1 La Ga1 103.25(3) 2_455 .
O1 La Ga1 103.25(3) . .
O2 La Ga1 69.21(17) . .
O2 La Ga1 69.21(17) 6 .
Ga2 La Ga1 100.041(15) . .
Ga2 La Ga1 100.042(15) 2_565 .
O3 La Ta 33.66(18) 6 .
O3 La Ta 33.66(18) . .
O2 La Ta 129.7(2) 2_455 .
O2 La Ta 129.7(2) 4_455 .
O1 La Ta 103.25(3) 2_455 .
O1 La Ta 103.25(3) . .
O2 La Ta 69.21(17) . .
O2 La Ta 69.21(17) 6 .
Ga2 La Ta 100.041(15) . .
Ga2 La Ta 100.042(15) 2_565 .
Ga1 La Ta 0.0 . .
O3 Ga1 O3 84.2(5) 2 3
O3 Ga1 O3 106.1(6) 2 4
O3 Ga1 O3 86.1(3) 3 4
O3 Ga1 O3 163.8(6) 2 .
O3 Ga1 O3 86.1(3) 3 .
O3 Ga1 O3 86.1(3) 4 .
O3 Ga1 O3 86.1(3) 2 5
O3 Ga1 O3 163.8(6) 3 5
O3 Ga1 O3 84.2(5) 4 5
O3 Ga1 O3 106.1(6) . 5
O3 Ga1 O3 86.1(3) 2 6
O3 Ga1 O3 106.1(6) 3 6
O3 Ga1 O3 163.8(6) 4 6
O3 Ga1 O3 84.2(5) . 6
O3 Ga1 O3 86.1(3) 5 6
O3 Ga1 La 42.1(2) 2 2
O3 Ga1 La 42.1(2) 3 2
O3 Ga1 La 98.1(3) 4 2
O3 Ga1 La 127.0(3) . 2
O3 Ga1 La 127.0(3) 5 2
O3 Ga1 La 98.1(3) 6 2
O3 Ga1 La 127.0(3) 2 .
O3 Ga1 La 98.1(3) 3 .
O3 Ga1 La 127.0(3) 4 .
O3 Ga1 La 42.1(2) . .
O3 Ga1 La 98.1(3) 5 .
O3 Ga1 La 42.1(2) 6 .
La Ga1 La 120.0 2 .
O3 Ga1 La 98.1(3) 2 4
O3 Ga1 La 127.0(3) 3 4
O3 Ga1 La 42.1(2) 4 4
O3 Ga1 La 98.1(3) . 4
O3 Ga1 La 42.1(2) 5 4
O3 Ga1 La 127.0(3) 6 4
La Ga1 La 120.0 2 4
La Ga1 La 120.0 . 4
O3 Ta O3 84.2(5) 2 3
O3 Ta O3 106.1(6) 2 4
O3 Ta O3 86.1(3) 3 4
O3 Ta O3 163.8(6) 2 .
O3 Ta O3 86.1(3) 3 .
O3 Ta O3 86.1(3) 4 .
O3 Ta O3 86.1(3) 2 5
O3 Ta O3 163.8(6) 3 5
O3 Ta O3 84.2(5) 4 5
O3 Ta O3 106.1(6) . 5
O3 Ta O3 86.1(3) 2 6
O3 Ta O3 106.1(6) 3 6
O3 Ta O3 163.8(6) 4 6
O3 Ta O3 84.2(5) . 6
O3 Ta O3 86.1(3) 5 6
O3 Ta La 42.1(2) 2 2
O3 Ta La 42.1(2) 3 2
O3 Ta La 98.1(3) 4 2
O3 Ta La 127.0(3) . 2
O3 Ta La 127.0(3) 5 2
O3 Ta La 98.1(3) 6 2
O3 Ta La 127.0(3) 2 .
O3 Ta La 98.1(3) 3 .
O3 Ta La 127.0(3) 4 .
O3 Ta La 42.1(2) . .
O3 Ta La 98.1(3) 5 .
O3 Ta La 42.1(2) 6 .
La Ta La 120.0 2 .
O3 Ta La 98.1(3) 2 4
O3 Ta La 127.0(3) 3 4
O3 Ta La 42.1(2) 4 4
O3 Ta La 98.1(3) . 4
O3 Ta La 42.1(2) 5 4
O3 Ta La 127.0(3) 6 4
La Ta La 120.0 2 4
La Ta La 120.0 . 4
O1 Ga2 O2 117.7(3) 2_456 5_445
O1 Ga2 O2 117.7(3) 2_456 2_455
O2 Ga2 O2 100.2(3) 5_445 2_455
O1 Ga2 O2 117.7(3) 2_456 6
O2 Ga2 O2 100.2(3) 5_445 6
O2 Ga2 O2 100.2(3) 2_455 6
O1 Ga2 La 134.58(2) 2_456 4_445
O2 Ga2 La 56.8(3) 5_445 4_445
O2 Ga2 La 107.3(3) 2_455 4_445
O2 Ga2 La 43.4(3) 6 4_445
O1 Ga2 La 134.58(2) 2_456 .
O2 Ga2 La 107.3(3) 5_445 .
O2 Ga2 La 43.4(3) 2_455 .
O2 Ga2 La 56.8(3) 6 .
La Ga2 La 76.18(4) 4_445 .
O1 Ga2 La 134.58(2) 2_456 2_455
O2 Ga2 La 43.4(3) 5_445 2_455
O2 Ga2 La 56.8(3) 2_455 2_455
O2 Ga2 La 107.3(3) 6 2_455
La Ga2 La 76.18(4) 4_445 2_455
La Ga2 La 76.18(4) . 2_455
O3 Ga3 O3 132.6(6) 4_454 2_455
O3 Ga3 O2 109.2(4) 4_454 4_455
O3 Ga3 O2 100.3(4) 2_455 4_455
O3 Ga3 O2 100.3(4) 4_454 2_454
O3 Ga3 O2 109.3(4) 2_455 2_454
O2 Ga3 O2 101.5(6) 4_455 2_454
Ga2 O1 La 110.5(2) 2_566 2_565
Ga2 O1 La 110.5(2) 2_566 .
La O1 La 108.4(2) 2_565 .
Ga2 O1 La 110.5(2) 2_566 4_455
La O1 La 108.4(2) 2_565 4_455
La O1 La 108.4(2) . 4_455
Ga2 O2 Ga3 119.0(5) 2_565 2_564
Ga2 O2 La 105.5(4) 2_565 2_565
Ga3 O2 La 120.1(4) 2_564 2_565
Ga2 O2 La 90.8(3) 2_565 .
Ga3 O2 La 111.7(4) 2_564 .
La O2 La 105.2(3) 2_565 .
Ga3 O3 Ta 113.8(5) 2_565 .
Ga3 O3 Ga1 113.8(5) 2_565 .
Ta O3 Ga1 0.0 . .
Ga3 O3 La 137.9(4) 2_565 .
Ta O3 La 104.3(3) . .
Ga1 O3 La 104.3(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.409(9) 6
La O3 2.409(9) .
La O2 2.432(9) 2_455
La O2 2.432(9) 4_455
La O1 2.593(4) 2_455
La O1 2.593(4) .
La O2 2.853(10) .
La O2 2.853(10) 6
La Ga2 3.4098(14) .
La Ga2 3.4098(14) 2_565
La Ga1 3.4844(8) .
La Ta 3.4844(8) .
Ga1 O3 1.993(8) 2
Ga1 O3 1.993(8) 3
Ga1 O3 1.993(8) 4
Ga1 O3 1.993(8) .
Ga1 O3 1.993(8) 5
Ga1 O3 1.993(8) 6
Ga1 La 3.4844(8) 2
Ga1 La 3.4844(8) 4
Ta O3 1.993(8) 2
Ta O3 1.993(8) 3
Ta O3 1.993(8) 4
Ta O3 1.993(8) .
Ta O3 1.993(8) 5
Ta O3 1.993(8) 6
Ta La 3.4844(8) 2
Ta La 3.4844(8) 4
Ga2 O1 1.797(12) 2_456
Ga2 O2 1.826(9) 5_445
Ga2 O2 1.826(9) 2_455
Ga2 O2 1.826(9) 6
Ga2 La 3.4097(14) 4_445
Ga2 La 3.4098(14) 2_455
Ga3 O3 1.822(8) 4_454
Ga3 O3 1.822(8) 2_455
Ga3 O2 1.878(8) 4_455
Ga3 O2 1.878(8) 2_454
O1 Ga2 1.797(12) 2_566
O1 La 2.593(4) 2_565
O1 La 2.593(4) 4_455
O2 Ga2 1.826(9) 2_565
O2 Ga3 1.878(8) 2_564
O2 La 2.432(9) 2_565
O3 Ga3 1.822(8) 2_565
